Journal of Global Resources
Biannual International Peer-Reviewed Journal
ISSN: 2395-3160 (Print)/2455-2445 (Online)

January 2021
Volume 07 (01)
Crossref DOI 10.46587

DOI: 10.46587/JGR.2021.v07i01.019

19
CHITOSAN Fe2O3 NANO COMPOSITES COMPETENT FOR REMOVAL OF HEAVYMETAL WATER POLLUTANT’S (Hg+2, Co+2, Ni+2)
Imtiyaz Rasool Parrey* and Hilal Ul Zaman
Govt. Degree College for Women, Anantnag, Jammu and Kashmir, India*Corresponding author Email: imtiyazchemsitry@gmail.com

Abstract: In this examination, novel chitosan/Fe2O3 nanocomposite was incorporated andevaluated as an adsorbent for expelling thorium (IV) particles from the fluid arrangement.
The Ch/Fe- nanocomposites were labeled by x-ray diffraction (XRD), Brunauer–Emmett–Teller (BET) Fourier Transform Infrared Spectroscopy (FT-IR) and Scanning electron
microscopy (SEM). The most elevated Hg2+ evacuation yield was seen as 99.3 percent
utilizing the 2:1 (w/w) nanocomposite at pH 6 out of 100 ppm of Hg 2+ arrangement. The Ni2+expulsion yield was seen as 98.5 percent utilizing the 2:1 (w/w) nano composite at pH
5.5 in 100 ppm of Hg+2. The Co2+ expulsion yield was 98.7 percent at pH 5.5 in 60 ppmof Co2+ arrangement utilizing the 4:1 (w/w) nanocomposite.
Key words: Chitosan/Fe2O3, Adsorbent, XRD, FT-IR
Introduction
Nanotechnology is viewed as a novel innovation that is advancing quickly and spreading
its application spaces in all measurements. Nanotechnology incorporates development,
assessing, and controlling issue at the nuclear, sub-atomic, macromolecular, and micro
molecular scales, with the end goal that the subsequent material has one of a kind andvarious properties from the parent mass material (Bhatt and Tripathi, 2011; Khan, Mobin,Abbas, AlMutairi, and Siddiqui, 2017). The particles created through this are named as
designed nanoparticles (ENPs) or essentially nanoparticles (NPs). ENPs are characterized
as particles having, at any rate, one outside measurement somewhere in the range of 1and 100nm (Shi, Abid, Kennedy, Hristova, and Silk, 2011; Thuesombat, Hannongbua,
Akasit, and Chadchawan, 2014). Nanotechnology discovers applications in a broad scopeof segments extending from agribusiness, food creation and bundling, clinical symptomatic,pharmaceutical, the nano-based epitome of pesticides, hereditary material conveyance inplants, sedate conveyance in people, and malignant growth treatment to some more (DeOliveira, Campos, Bakshi),
Abhilash & Fraceto, 2014; Ghormade et al., 2011; Gogos, Knauer, & Bucheli, 2012).
Besides these, its most anticipated applications have been for remediation ofenvironmental compartments like water and soil [1-5]. These fuse treatment of wastewater,
cleaning of groundwater, and remediation of soil polluted with harms (Karn, Kuiken, andOtto, 2009; Kuiken, 2010; Rogueda and Traini, 2007; Roh, Park, Park, and Choi, 2010; Shi,Votruba, Farokhzad, and Langer, 2010). Manganese Oxides-Based Nanomaterials
Manganese oxides nanoparticles have additionally been accounted for to expel substantial
metals from wastewater and Nano sized manganese dioxide just as hydrous manganeseoxide (HMO) in which Mn is quadrivalve are for the most part talked about here. Nano
crystalline manganese oxide was found to have a high surface region which adds to its
great adsorption execution. Wang et al. blended a novel free weight like manganesedioxide/gelatin and examined its adsorption exhibitions towards Pb (II) and Cd (II) [6-8].
The cluster adsorption study demonstrated that the most extreme adsorption limits towards
150Pb (II) and Cd (II) were 318.7 and 105.1 mmol.g-1 individually by figuring from the Langmuirmodel. The adsorption motor followed the pseudo-second-request model. Also, thisnanocomposite could be exploited to treat genuine water in the wake of being upheld on
an amino-functionalized PMMA plate. High expulsion limit, straightforward activity, andgreat dependability inferred that this nanocomposite could be applied to rewarding
overwhelming metals in genuine water. Moreover, nanoscale manganese dioxide could
likewise be utilized in the adsorption and oxidation of Tl (I) in wastewater [8-10]. This groupadsorption procedure could be done in 15 min and the greatest evacuation limit wasdetermined to be 672 mg.g-1 by utilizing the Langmuir model, showing the capability ofnanosized manganese oxides to be utilized in Tl treatment. What's more to these metals,
manganese oxides-based nanomaterials have additionally been accounted for to treat
other overwhelming metals like U, Cd(II), Cu(II), Pb(II), Zn(II), Hg (II, etc. [11-13]. Hydrous
manganese oxide (HMO) is another sort of manganese oxides that have indicated its points
of interest in overwhelming metals evacuation thinking about its high surface region,
permeable structures, and plenteous destinations for adsorption. The coordination science
likewise assumes a noteworthy job in adsorption of HMO since hydroxyl bunches on theHMO surface could facilitate with substantial metal particles [14]. The adsorption ofsubstantial metal particles onto HMO was typically involved in two stages: the snappy
adsorption of overwhelming metals onto the outer surface and the moderate intra-molecule
dissemination along with the small scale pore dividers of HMO. As of late, wan et al.
arranged an HMO-BC nanocomposite by impregnating the HMO nanoparticles into thebiochar (BC) [15]. HMO-BC nanocomposite showed a brilliant expulsion impact towards Pb(II) and Cd (II) in a wide scope of pH. The mix of HMO and BC could maintain a strategic
distance from the disadvantages of utilizing BC exclusively, for example, the unacceptable
adsorption limit and poor selectivity [16-18]. Fixed-bed segment adsorption tests exhibitedthat the powerful treatment capacity of HMO-BC for a recreated Pb (II) or Cd (II) [19-21]
containing wastewater was around 4-6 times higher than that of the BC have.
Consequently, HMO-BC is a promising option for evacuating overwhelming Metals fromcontaminated water. Natural Polymer-Supported Nanocomposites Polymeric hosts havenumerous unprecedented properties, for example, magnificent mechanical quality [22-23].
Synthesis of Chitosan Fe2O3 Nano Composites
Everything the chosen reagents were of analytical grade and purchased from Merck. Thestock solutions for preparation of Co+2 , Hg +2 , Ni +2 were prepared by dissolving respective
metal salt in deionized water. The starter pH of arrangements was estimated by nitriccorrosive (HNO3; 99.9 percent) or sodium hydroxide (NaOH; 99.9 percent) arrangementsand Metrohm pH meter model 744. Sartorius Electrical Balance Model BP 221S,Nabertherm heater and blender HT Infors AG model CH-4103-BOT were utilized to direct
the investigations. Blend of adsorbent was finished by utilizing aqueous reactor, which wasstructured and made of treated steel 316 L just as traditional autoclaves with Teflon liner
by volume of 100 mL.
Amalgamation of Fe2O3 Nano molecule (Fe-ONPs) Fe-ONPs were set up by
aqueous combination strategy. One gram of FeCl3.6H2O, 3.5 g of hexa-methylene diamineand 1.5 g of trisodium citrate were broken down in 100 mL of refined water at a temperatureof 70 C and blended for 1 h. The arrangement was filled aqueous reactor and put inaqueous autoclave at 200 C for 10 h. The delivered Fe-ONPs were washed with deionizedwater and dried at room temperature. A blend of water and ethanol (1:5 (v/v)) was added
dropwise to the suspensions of FeONPs under incredible attractive mixing and left to makedue with 1 h. The altered Fe-ONPs was washed with refined water a few times and driedin the stove at 110 C for 3 h.
Combination of Ch/Fe-Onc Ch medium atomic load with the level of deacetylation
somewhere in the range of 75 and 85 percent was utilized so as to get ready Ch/Fe-Onc.
Ch (1.67 g) was broke up in 50 mL of 0.1 N hydrochloric corrosive arrangement andblended for 1 h. At that point 0.1 g of arranged Fe-ONPs was completely scattered in the151

Ch arrangement followed by the expansion of hydrochloric corrosive arrangement. Sampler
was utilized to trickle out the subsequent arrangement into 0.1 N sodium hydroxidearrangements. Beads were shaped as circular Nano composites with a breadth of 0.45 cm.
The subsequent Ch/Fe-Onc was kept up in sodium hydroxide answer for 24 h and, at last,
washed with deionized water and dried at room temperature. Subjective synthetic structureassessment was done by means of Fourier change infrared (FTIR) investigation (Vector22
Brucker Company, USA). Th4þ investigation was followed up by utilizing a Perkin-Elmer
Optima 2000 DV Model Inductively Coupled Plasma-Optic Emission Spectrometry (ICPOES)
X ray Diffraction
The XRD patterns of Ch/ Fe2O3 nanocomposites and its base materials (Ch/ Fe2O3 ) wererecorded using a Rigaku Ultima IV diffractometer with Hg +2 Kα (λ = 0.2189 nm) radiation.
The diffraction intensities were recorded from 5 to 40° (2θ) angle. The d spacing of MMTlayers was calculated using the Bragg equation
Figure 01: XRD patterns of (a) Fe- Ch nono composite (b) Fe- Ch nanocomposite(1:1), (c) Fe- Ch nonocomposite (2:1), (d) Fe- Ch noncomposite (4:1)

SEM Analysis
SEM analyses of Nano composite samples were carried out on a Sigma HD Zeuss
scanning electron microscope at an acceleration voltage of 20 kV (SE detector). The main
objective of this characterization technique is the identification of materials morphology thatrepresents a key factor to analyze in the adsorption process.
Figure 02: SEM micrographs of (a) Fe- Ch nanocomposite (b) Fe- Ch
nanocomposites (c) Fe- Ch nanocomposites (d) Fe- Ch nanocomposites

152

Adsorption Study Report
Adsorption Isotherms Conclusion
Adsorption is an active process that is usually defined by isotherms, determined by fitting
mathematical models to experimental data. The information provided by these models
quantifies how the adsorbate is distributed between the solid and liquid phases. In thisinvestigation, the Langmuir, eq 1, and the Freundlich, isotherms were used to study theequilibrium adsorption of Hg+2 (1:1), Co2+ (2:1) and Ni2+ ions onto Ch/ Fe2O3
nanocomposites (4:1 w/w). The suitability of both models was quantified with the correlation
factor (R2) obtained from linear fitting and adsorption capacity constant (qe).
(1)
In qe = In K1+ 1/n In Ce (2)In eqs 1 and 2 qm is the amount of heavy metal present in a monolayer (mg/g), Ce is theequilibrium concentration of heavy metal remaining in the solution (mg/L), qe is the quantityof the heavy metal adsorbed by per unit of adsorbent at equilibrium (mg/g),
Absorption Studies
Isothermal Study
Comparing the correlation coefficients (R2) obtained by fitting the adsorption results with
the Langmuir and Freundlich isotherms for Hg+2, Co2+ and Ni2+, the Langmuir isotherm
provided a better description of the data than the Freundlich isotherm for pH values of 5,
5.5 and 6, but when the pH was 3, the Freundlich isotherm outperformed the Langmuirisotherm. This suggests that a monolayer adsorption process on homogeneous sites(described by the Langmuir isotherm) takes place in aqueous solutions with lower acidity.
At lower pH esteems, the Langmuir model may go amiss from the genuine adsorption
conduct because of the presumption of no cooperations between sorbate particles. By theby, this model gives palatable understandings of a wide number of tests that predominantly
present chemisorption. Then again, the Freundlich isotherm models multilayer adsorption
forms on heterogeneous surfaces, and its better fit recommend that this component depicts
the procedure at pH 3 all the more precisely.
Figure 03: Substantial metal adsorption on Nano composite at pH values ofCh/Fe2O3(1:1) and Ni2+ ions, (b) (2:1) and Co2+ ions, (c) Ch/ Fe2O3 (4:1) and Hg2+ ions,(d) Ch/ Fe2O3 (1:1).

153

Figure 04: RL dimensionless factor versus initial concentration for (a) Hg2+ ions and(b) Ni2+ ions and (c) Co2+ at pH estimations of 5 and 6 with the Ch/ Fe2O3Conclusion
This exploration scheme assessed the adsorption limit of nanocomposites dependent on
Ch/Fe2O3 for the expulsion of overwhelming metal particles (Hg2+, Ni2+ and Co2+) fromwastewater. SEM and XRD to evaluate utilitarian gatherings, morphologies, and structuresdescribed the readied composites. Adsorption of Hg 2+, Ni2+ and Co2+ particles is best
depicted by the Langmuir isotherm at higher pH esteems, as prove by a coefficient ofrelationship near one.
References
1. Abdullah, J.A., Lafi, A.G.A., Amin, Y., Alnama, T. A. (2013). Styrofoam-nanomanganese oxide based composite:168. Mukherjee, J.; Ramkumar, J.; Shukla, R.;
Tyagi, A.K. Sorption characteristics of nano manganese oxide: Efficient sorbent forremoval of metal ions from aqueous streams. J. Radioanal. Nuclear Chem, 297, 49–57
2. Abdullah, J.A., Lafi, A.G.A.; Amin, Y.; Alnama, T. A. (2018). Styrofoam-nanomanganese oxide based composite: Preparation and application for the treatment ofwastewater. Appl. Radiat. Isotopes, 136, 73.
3. Anandan, S., Kathiravan, K., Murugesan, V., Ikuma, Y. (2009). Anionic IO3- non-metaldoped TiO2 nanoparticles for the photocatalytic degradation of hazardous pollutant inwater. Catal. Commun. 10, 1014–1019.
4. Byungryul, A., Steinwinder, T.R., Dongye, Z. (2017). Selective removal of arsenate fromdrinking water using apolymeric ligand exchanger. Water Res. 2005, 39, 4993–5004.166. Huo, L.; Zeng, X.; Su, S.; Bai, L.; Wang, Y. Enhanced removal of as (V) from
aqueous solution using modified hydrous ferric oxide nanoparticles. Sci. Rep., 7, 40765.
5. Fan, M., Boonfueng, T.; Xu, Y.; Axe, L., Tyson, T.A. (2005). Modeling Pb sorption tomicroporous amorphous oxides as discrete particles and coatings. J. Colloid Interface
Sci., 281, 39–48
6. Ghiloufi, I., Mir, L.E. (2015). Preparation and characterization of nanoporous resin forheavy metal removal from aqueous solution. J. Water Supply Res. Technol.-Aqua, 64,316–325.

154

7. Hadadian, M., Goharshadi, E.K., Fard, M.M., Ahmadzadeh, H. (2018). Synergistic
effect of graphene nanosheets and zinc oxide nanoparticles for effective adsorption ofNi(II) ions from aqueous solutions. Appl. Phys. A, 124, 239.
8. Huangfu, X., Jin, J., Lu, X., Wang, Y., Liu, Y., Pang, S.Y., Cheng, H., Xiang, Z., Ma,J. (2015). Adsorption and Oxidation of Thallium(I) by a Nanosized Manganese Dioxide.
Water Air Soil Pollut. 226, 2272.
9. Huangfu, X., Jin, J., Lu, X., Wang, Y, Liu, Y., Pang, S.Y., Cheng, H., Xiang, Z., Ma,J. (2015). Adsorption and Oxidationof Thallium(I) by a Nano sized Manganese Dioxide.
Water Air Soil Pollute.226, 2272.
10. Hui, Q., Shujuan, Z., Bingcai, P., Weiming, Z., Lu, L. (2012). Effect of sulfate on Cu(II)sorption to polymer-supported nano-iron oxides: Behavior and XPS study. J. ColloidInterface Sci. 2012, 366, 37–43.162.
11. Singh, S.K., Subramanian, V., Gibbs, R.J. (1984). Hydrous FE and MN oxides—
Scavengers of heavy metals in the aquatic environment. Crit. Rev. Environ. Control,14, 33–90.
12. Hui, Q., Zhang, S., Pan, B., Zhang, W., Lu, L. (2013). Oxalate-promoted dissolution ofhydrous ferric oxide immobilized within nano porous polymers: Effect of ionic strengthand visible light irradiation. Chem. Eng. J., 232, 167–173.
13. Kumar, K.Y., Muralidhara, H.B., Nayaka, Y.A., Balasubramanyam, J., Hanumanthappa,H. (2013). Low-cost synthesis of metal oxide nanoparticles and their application inadsorption of commercial dye and heavy metal ion in aqueous solution. Powder
Technol., 246, 125–136.
14. Lisha, K.P.; Maliyekkal, S.M.; Pradeep, T. (2010). Manganese dioxide nano whiskers:
A potential adsorbent for the removal of Hg(II) from water. Chem. Eng. J., 160, 432–439.
15. Lockwood, R.A., Chen, K.Y. (1973). Adsorption of mercury(II) by hydrous manganeseoxides. Environ. Sci. Technol, 7, 1028–1034.
16. Mukherjee, J., Ramkumar, J., Shukla, R., Tyagi, A.K. (2013). Sorption characteristicsof nano manganese oxide: Efficient sorbent for removal of metal ions from aqueousstreams. J. Radioanal. Nuclear Chem, 297,49–57.
17. Rafiq, Z., Nazir, R., Durr-e-Shahwar; Shah, M.R., Ali, S. (2014). Utilization ofmagnesium and zinc oxide nano-adsorbents as potential materials for treatment ofcopper electroplating industry wastewater. J. Environ. Chem. Eng., 2, 642–651.
18. Sheela, T., Nayaka, Y.A., Viswanatha, R., Basavanna, S.. Venkatesha, T.G. (2012).
Kinetics and thermodynamics studies on the adsorption of Zn(II), Cd(II) and Hg(II) from
aqueous solution using zinc oxide nanoparticles. Powder Technol, 217, 163–170.
19. Somu, P.; Paul, S. (2018). Casein based biogenic-synthesized zinc oxide nanoparticles
simultaneously decontaminate heavy metals, dyes, and pathogenic microbes: A
rational strategy for wastewater treatment. J. Chem. Technol. Biotechnol.
20. Sposito, G.(1983). On the surface complexation model of the oxide-aqueous solution
interface. J. Colloid Interface Sci., 91, 329–340.
21. Wan, S., Wu, J., Zhou, S., Rui, W., Gao, B.,Feng, H. (2018). Enhanced lead andcadmium removal using biochar-supported hydrated manganese oxide (HMO)
nanoparticles: Behavior and mechanism. Sci. Total Environ, 616–617, 1298–1306.
22. Wang, X., Huang, K., Chen, Y., Liu, J., Chen, S., Cao, J., Mei, S., Zhou, Y., Jing, T.
(2018). Preparation of dumbbell manganese dioxide/gelatin composites and theirapplication in the removal of lead and cadmium ions. J. Hazard. Mater, 350, 46–54.
23. Wang, X. Huang, K., Chen, Y., Liu, J.; Chen, S., Cao, J., Mei, S.; Zhou, Y., Jing, T.
(2018). Preparation of dumbbell manganese dioxide/gelatin composites and theirapplication in the removal of lead and cadmium ions. J. Hazard. Mater.350, 46–54
24. Zhang, Y. Li, Z. (2017). Heavy metals removal using hydrogel-supported nanosizedhydrous ferric oxide: Synthesis, characterization, and mechanism. Sci. Total Environ.,
580, 776–786.

155